This article needs additional citations for verification. (December 2016) (Learn how and when to remove this template message)
The water–cement ratio is the ratio of the weight of water to the weight of cement used in a concrete mix. A lower ratio leads to higher strength and durability, but may make the mix difficult to work with and form. Workability can be resolved with the use of plasticizers or super-plasticizers.
Often, the ratio refers to the ratio of water to cementitious materials, w/cm. Cementitious materials include cement and supplementary cementitious materials such as fly ash, ground granulated blast-furnace slag, silica fume, rice husk ash and natural pozzolans. Supplementary cementitious materials are added to strengthen concrete.
The notion of water–cement ratio was first developed by Duff A. Abrams and published in 1918. Refer to concrete slump test. The 1997 Uniform Building Code specifies a maximum of 0.5 ratio when concrete is exposed to freezing and thawing in a moist condition or to de-icing chemicals, and a maximum of 0.45 ratio for concrete in a severe or very severe sulfate condition.
Concrete hardens as a result of the chemical reaction between cement and water (known as hydration, this produces heat and is called the heat of hydration). For every pound (or kilogram or any unit of weight) of cement, about 0.35 pounds (or 0.35 kg or corresponding unit) of water is needed to fully complete hydration reactions.
However, a mix with a ratio of 0.35 may not mix thoroughly, and may not flow well enough to be placed. More water is therefore used than is technically necessary to react with cement. Water–cement ratios of 0.45 to 0.60 are more typically used. For higher-strength concrete, lower ratios are used, along with a plasticizer to increase flowability.
Too much water will result in segregation of the sand and aggregate components from the cement paste. Also, water that is not consumed by the hydration reaction may leave concrete as it hardens, resulting in microscopic pores (bleeding) that will reduce final strength of concrete. A mix with too much water will experience more shrinkage as excess water leaves, resulting in internal cracks and visible fractures (particularly around inside corners), which again will reduce the final strength.
- Somayaji, Shan (2001). Civil Engineering Materials. Upper Saddle River: Prentice Hall. p. 129. ISBN 0-13-083906-X.
The water-to-cement ratio is the ratio between the weights of water and cement in a concrete mix. For proper hydration, this ratio (commonly called the w/c ratio) should be about 0.30, assuming no contribution to hydration from external water sources.